**IJEEE, Volume 3, Issue 1 (February 2016)** **e-ISSN: 1694-2310 | p-ISSN: 1694-2426**

**ESTIMATION OF BREAKDOWN**

**STRENGTH OF SOLID INSULATING**

**MATERIALS**

**A. Masood**

**1**

**, M.U. Zuberi**

**2**1,2

Department of Electrical Engineering, Aligarh Muslim University, Aligarh, India 2

mu.zuber.ee@amu.ac.in

**Abstract-The objective of this research was to correlate**

**dielectric strength (E) of electrical insulating materials**
**with other properties like volume resistivity (v),**
**relative permittivity (r), loss tangent (tan) and**
**thickness (t) on an empirical basis. A simple equation**
**of the form E=A + Blog (v** **/rtan) to predict the**
**dielectric strength of a solid insulating material in the**

**ambient medium has been proposed. The constant ‘B’**

**has been obtained as a function of thickness (t) of solid**
**insulating materials. The values of electric strength**
**calculated using this equation for Polyethylene, Nomex,**
**Leatheroid, Trivoltherm, Clasefleece and Polyethylene**
**coated Leatheroid are quite in agreement with the**

**experimentally ** **measured values. The ** **proposed**

**equation is subsequently verified by calculating the**
**electric strength of Kraft paper, Mica, Empire cloth**
**and Fiber glass and is found to be quite in agreement**
**with earlier reported results. It is expected that the**
**equation obtained will help the designers as a handy**
**tool for quick estimation of breakdown strength of**
**solid dielectrics.**

**Index Terms- Breakdown Strength, Loss Tangent,**

Relative Permittivity, Solid Dielectrics, Volume Resistivity

**I.** **INTRODUCTION**

Solid insulating materials form an integral part of all electrical equipment especially when the operating voltages are high. The design of any electrical apparatus is based on the dielectric strength of the electrical insulation used and the design cannot be completely relied upon unless an assessment of the dielectric strength of insulation against applied voltages is made using high voltage testing.

When high voltage testing is done on component parts, elaborate insulation assemblies, and complete full-scale prototype apparatus, it is possible to build up a considerable stock of design information. Such test data, although expensive, can be very useful, but it can never really be complete to cover all future designs and necessitates use of large factors of safety. A different approach to the problem is the estimation of dielectric strength of the insulation arrangement.

The theory behind dielectric breakdown has not been fully understood. The interaction of fields, particles and atoms on a microscopic level is so complex that exact quantum mechanical solution is simply not possible [1,2].

A number of factors affecting dielectric strength, could be listed and evaluated [3-5]. These include intrinsic material properties, external environmental factors and test conditions that may exist.However, the list can be shortened considerablyif the environmental factors and test conditions are kept constant. If this were the case, then a list of intrinsic material properties which might affect the dielectric strength such as relative permittivity (r), loss tangent (tan),sample thickness (t), mobility of charge carriers (), numberof charge carriers (n), ionization energy (Ei),free path among molecules () and free volume of the material (Vf) would result [6,7].

Out of the above parameters r, tan and t can be measured in a relatively straight forward manner. Mobility of charge carriers is very difficult to define [8]. However, if the number of charge carriers are known, the volume resistivity (v) measurement can be used to determine through the equationv=1/ne.

Since the mean free path of a free electron in a material is dependent upon the free volume and the molecular agitation within the material, which are themselves temperature dependent, the increase in free volume with temperature leads to an increase in the mean free path. However, the increased molecular agitation at high temperatures tends to decrease this path. Thus, the measurement and calculation of this parameter is most difficult.

Furthermore, from the energy considerations, the kinetic energy which an electron acquires when subjected to an electric field is dependent upon the mean free path between collisions, which in turn should be equal to the cube root of the free volume Vf.

With these constraints in measuring the above listed intrinsic properties, Swanson et al [6] suggested a relationship given by equation (1) to correlate the E with v,rand tan.

Dielectric Strength, E=A+Blog (v/rtan) --- (1) This is based on the assumption of performing experiments on the test samples of same thickness, which is again an approximation to eliminate thickness ‘t’ from the above equation.

deficiency of Eq. (1), the breakdown strength (BDS),
relative permittivity (r), loss tangent (tan) and thickness
(t) of different solid insulating materials in the ambient
medium have been measured and correlated incorporating
the thickness of the samples in the constant ‘B’to estimate
the BDS of solid insulants. The results obtained by the
proposed equation for Polyethylene, Nomex, Leatheroid,
Trivoltherm, Clasefleece and Polyethylene coated
Leatheroid were quite in agreement with the
**experimentally measured values [9] and the results are**
reproduced. Subsequently, the breakdown strength of
**earlier reported samples [10] for Kraft paper, Mica,**
Empire cloth and Fiber glass has been estimated using the
proposed equation and compared with the experimental
values.

**II. EXPERIMENTAL TECHNIQUES**

*A. Measurement of Relative Permittivity and Loss*
*Tangent of Solid Dielectrics*

Figure 1 shows the three-electrode system as described in [11] to measure the relative permittivity and loss tangent of various dielectrics. Measurements were made using Automatic Capacitance & Dissipation Factor test systemPE-ACDF-1 as shown in Figures 2. Its user-friendly GUI, along with its settings allows display of results on the same back-lighted colored LCD display and printed by an integrated panel printer.Measurement of r and tan were carried on Polyethylene, Nomex, Leatheroid, Trivoltherm, Clasefleeceand Polyethylene

coated Leatheroid.

(a) Schematic of three electrode system

### EXPERIMENTAL SETUP

(a) PE-ACDF-1Front Panel

(b) Experimental Test Cell with PE-ACDF-1

Figure 2

*B. Breakdown Strength Of Solid Dielectrics*

Trivoltherm, Clasefleeceand Polyethylene coated Leatheroid in any way since it was assumed that any contaminants such as ionic impurities which would influence the dielectric strength would also influence other properties being measured. Thus the materials were tested as received in the laboratory.

The sample thickness was measured at some randomly distributed 20 points, spread all over the sheet area with a micrometer having a least count of 0.01mm. The average of the 20 measurements was taken as the average thickness of the sample.

**III.RESULTS**

Volume resitivities of the materials were not measured practically but noted from the literature available [13-15].

Collecting all relevant data for different insulating material samples, log (v/rtan) was calculated for each of them. Samples were grouped together according to thickness and for each group measured electric strength was plotted against the quantity log (v/rtan).

The plot is as shown in Figure 4. For thick samples the slope of straight line is lesser than the slope for thin samples and these decreases in a regular fashion.

Equations (2) to (5) plotted in Figure 4 are for four thickness groups of samples [0.1-0.3mm, 0.31-0.5mm, 0.51-0.7mm and 0.71-0.9mm].

E1= -22.09+4.853 log (v/rtan) ---(2)

E2= -20.18+4.500 log (v/rtan)---(3)

E3= -18.73+4.213 log (v/rtan)---(4)

E4 = -15.65+3.840 log (v/rtan)---(5)

Thus all the measured data can be put in the form of an equation E= -A+B log (v/rtan) --- (6)

Considering the mean value of a particular range of
thickness of samples, it was observed that that constant
‘B’ is inversely related to thickness‘t’ of the sample.
Figure 5 shows a plot between ‘B’ values versus
thickness‘t’ of sample which is again a straight line and
mathematically expressed as
B= 5.1835-1.6627(t)
Thus final equation (6) may be expressed as
E = -19.165+ (5.1835-1.6627t) log (v/rtan**)---- (7)**

Here 19.165 is the average of ‘A’ values of Eqs. (2)- (5).

The calculated values using eqs (7) and measured values of electric strength of various solid insulating materials mentioned earlier are listed in Table 1. Errors in most of the cases are within ± 10 %.[9]

Figure 5. Constant ‘B’ vs. thickness‘t’ curve

Using the same proposed equation (7) the breakdown strength of earlier reported samples [10] was estimated for Kraft paper, Mica, Empire cloth and Fiber glass and the results are found to be within±10% error and are as shown in Table 2.

**IV.** **CONCLUSION**

Empirical formula suggested as given by Eq (7) for estimation of electric strength of solid insulating material is simple and gives results with errors within 10% and is thus valid provided thickness is small as can be seen from Tables 1&2. It is expected that the equation obtained will help the designers as a handy tool for quick estimation of breakdown strength of solid dielectrics.

TABLE1. ESTIMATION OF ELECTRIC STRENGTH OF SOLID INSULATING MATERIALS WITH PERCENTAGE ERROR.

Material

Density (g/cm3)

Dielectric Constant

r)

Dissipation Factor (tan)

Log[(v)/ rtan]

Thickness ‘t’ mm Measured E (kV/mm) Calculated E (kV/mm) % Error Polyethylene

ρv=2.1x10 16

Ωcm 1.0634

2.5202 0.0413 17.3048 0.19 65.789 65.068 1.00 2.5257 0.0473 17.2449 0.39 61.025 59.041 3.25 2.5763 0.0509 17.2045 0.58 56.206 53.423 4.90 2.6029 0.0532 17.1809 0.79 52.025 47.324 9.00

Leatheroid

ρv=1.6×1010Ωcm 0.9989

2.526 0.2019 10.4965 0.17 31.760 32.276 1.60

2.636 0.2051 10.4712 0.35 30.857 29.019 5.95

2.990 0.2131 10.3998 0.52 28.077 25.75 8.28

Nomex

ρv= 1×1014Ω cm

1.1226 2.493 0.092 14.6395 0.57 40.175 42.844 6.60

2.687 0.125 14.4738 0.76 38.158 37.570 1.50

Trivoltherm

ρv= 1.5×1015Ω cm _{1.1287}

2.083 0.1410 15.7081 0.23 57.826 56.251 2.70

2.194 0.1608 15.6286 0.45 53.111 50.153 5.50

2.309 0.1786 15.5608 0.69 48.695 43.63 10.3

Polyethylene Coated Leatheroid

ρv= 3.4×10 11

Ωcm

1.0594

2.497 0.1311 12.0165 0.19 36.842 39.326 6.80

2.555 0.1330 12.0002 0.39 32.307 35.25 9.13

2.592 0.1346 11.9887 0.56 30.357 31.81 4.8

2.648 0.1396 11.9636 0.77 29.221 27.532 5.70

Clasefleece

ρv=1×1013Ω cm 1.1481

2.348 0.0191 14.3483 0.66 38.636 39.464 2.10

2.419 0.0198 14.3196 0.87 36.552 34.347 6.00

TABLE 2VERIFICATION OF THE PROPOSED EQUATION

Material Loss index rtan)

Log[(v)/rtan] Thickness

‘t’ mm Measured E (kV/mm) Calculated E (kV/mm) % Error

Kraft Paper 0.903 08.74 0.41 18.53 20.18 8.90

Fiber Glass 0.028 14.20 0.16 46.25 50.66 9.54

Mica 0.035 16.07 0.20 55.00 58.78 6.89

Empire Cloth 0.051 15.02 0.15 50.00 54.94 9.89

Polyethylene Coated Leatheroid

0.015 13.32 0.27 40.00 43.89 9.74

Polyethylene 8.1x10-3 18.41 0.41 60.02 63.71 6.15

Leatheroid 0.200 10.90 0.15 32.00 34.61 8.17

**REFERENCES**

[1] A.K .Joncher, “*Dielectric relaxation in solids*”, Chelsea

Electromechanical and Power Systems, October 8-9, 2009 -Iaşi,

Romania.

[7] E. Husain, M.M. Mohsin and R.S. Nema, IEEE Electr. Insul. Dielectric. Phenomena (CEIDP), (1989) 453.

[8] J. Mort, 8th_{Symposium on Electr. Insul. , Japan (1975).}

[9] A. Masood, M.U.Zuberi et al “Breakdown Strength of Solid
Insulating Materials in Ambient Medium”3rd _{International}

Conference on Science, Technology & Management (ICSTM-2016), New Delhi, 17 January, 2016.

[10] A. Masood, M.U.Zuberi et al “Estimation of Breakdown Strength of Solid Insulating Materials in Ambient Medium”Invt. Journal of Science & Tech, Vol.6, No.1, 2013; pp.16-19. [11] E.W. Golding, Electrical Measurement and Measuring

Instruments, Wheeler Publication, London, (1980).

[12] IS: 2584-1963, “Method of Test for Electric strength of solid insulating materials at power frequencies”.

[13] Hippel, Dielectric Materials and Applications, The Technology Press of MIT, Wiley (1954).

[14] F.M. Clark, Insulating materials for design and Engineering Practice, Wiley, 1962.